### Delft University of Technology

### Idealized 3D auxetic mechanical metamaterial

### An analytical, numerical, and experimental study

Ghavidelnia, Naeim; Bodaghi, Mahdi; Hedayati, Reza DOI10.3390/ma14040993 Publication date 2021

Document Version Final published version Published in

Materials

Citation (APA)

Ghavidelnia, N., Bodaghi, M., & Hedayati, R. (2021). Idealized 3D auxetic mechanical metamaterial: An analytical, numerical, and experimental study. Materials, 14(4), 1-36. [993].

https://doi.org/10.3390/ma14040993 Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

Article

**Idealized 3D Auxetic Mechanical Metamaterial: An Analytical,**

**Numerical, and Experimental Study**

**Naeim Ghavidelnia1** **, Mahdi Bodaghi2** **and Reza Hedayati3,***

**Citation:** Ghavidelnia, N.; Bodaghi,
M.; Hedayati, R. Idealized 3D Auxetic
Mechanical Metamaterial: An
Analytical, Numerical, and
**Experimental Study. Materials 2021,**
14, 993. https://doi.org/10.3390/
ma14040993

Academic Editor: Antonio Santagata

Received: 5 January 2021 Accepted: 16 February 2021 Published: 20 February 2021

**Publisher’s Note:**MDPI stays neutral
with regard to jurisdictional claims in
published maps and institutional
affil-iations.

**Copyright:** © 2021 by the authors.
Licensee MDPI, Basel, Switzerland.
This article is an open access article
distributed under the terms and
conditions of the Creative Commons
Attribution (CC BY) license (https://
creativecommons.org/licenses/by/
4.0/).

1 _{Department of Mechanical Engineering, Amirkabir University of Technology (Tehran Polytechnic),}

Hafez Ave, Tehran 1591634311, Iran; n.ghavidelnia@aut.ac.ir

2 _{Department of Engineering, School of Science and Technology, Nottingham Trent University,}

Nottingham NG11 8NS, UK; mahdi.bodaghi@ntu.ac.uk

3 _{Novel Aerospace Materials, Faculty of Aerospace Engineering, Delft University of Technology (TU Delft),}

Kluyverweg 1, 2629 HS Delft, The Netherlands

***** Correspondence: r.hedayati@tudelft.nl or rezahedayati@gmail.com

**Abstract:**Mechanical metamaterials are man-made rationally-designed structures that present
un-precedented mechanical properties not found in nature. One of the most well-known mechanical
metamaterials is auxetics, which demonstrates negative Poisson’s ratio (NPR) behavior that is very
beneficial in several industrial applications. In this study, a specific type of auxetic metamaterial
structure namely idealized 3D re-entrant structure is studied analytically, numerically, and
experi-mentally. The noted structure is constructed of three types of struts—one loaded purely axially and
two loaded simultaneously flexurally and axially, which are inclined and are spatially defined by
*angles θ and ϕ. Analytical relationships for elastic modulus, yield stress, and Poisson’s ratio of the*
3D re-entrant unit cell are derived based on two well-known beam theories namely Euler–Bernoulli
and Timoshenko. Moreover, two finite element approaches one based on beam elements and one
based on volumetric elements are implemented. Furthermore, several specimens are additively
manufactured (3D printed) and tested under compression. The analytical results had good agreement
with the experimental results on the one hand and the volumetric finite element model results on the
other hand. Moreover, the effect of various geometrical parameters on the mechanical properties of
*the structure was studied, and the results demonstrated that angle θ (related to tension-dominated*
*struts) has the highest influence on the sign of Poisson’s ratio and its extent, while angle ϕ (related to*
compression-dominated struts) has the lowest influence on the Poisson’s ratio. Nevertheless, the
*compression-dominated struts (defined by angle ϕ) provide strength and stiffness for the structure.*
The results also demonstrated that the structure could have zero Poisson’s ratio for a specific range of

*θand ϕ angles. Finally, a lightened 3D re-entrant structure is introduced, and its results are compared*

to those of the idealized 3D re-entrant structure.

**Keywords:**3D printing; mechanical metamaterial; auxetics; negative Poisson’s ratio; 3D re-entrant

**1. Introduction**

The Poisson’s ratio is defined as the ratio of the negative value of transverse strain to the longitudinal strain of a body subjected to uniaxial stress [1]. The Poisson’s ratio is usually assumed to be positive (v > 0) for natural materials, which means that the material contracts transversely when stretched longitudinally or expands transversely when compressed longitudinally [2]. In contrast, there are some materials that reveal the opposite behavior of common materials and present negative Poisson’s ratio, which means that their transverse dimensions increase (or decrease) when they are subjected to axial tensile (or compressive) loads [3]. These materials have been given different names in the literature, including anti-rubber, dilational [4], and auxetic materials [5]. The term “auxetic” is currently the most widely accepted name used for materials with a negative Poisson’s ratio. Auxetic behavior has been observed in a few natural materials such as cristobalite

**Materials 2021, 14, 993** 2 of 36

(polymorphic silicones) [6], metals [7], zeolites [8], silicates [9,10], and some biological tissues such as cancellous bone [11], tendons [12], and some animal skins [13,14].

Mechanical metamaterials are man-made materials with unusual mechanical prop-erties and special functionalities not found in nature [15–19]. Negative Poisson’s ratio could be considered as one of such special mechanical properties [20–31]. Due to recent ad-vances in additive manufacturing techniques (3D printing), which provides the possibility of fabrication of rationally-designed materials with the desired accuracy in nano/micro-scale [32–35], the studies concentrated on design and analyzing auxetic metamaterials have been increasing exponentially during the last few years [36–40]. Different geometries with different deformation mechanisms have been introduced for auxetic structures. One of the first auxetic structures was proposed by Roberts [21], the first auxetic foam was presented by Lakes [41], and the first 2D molecular auxetic models (spontaneously forming auxetic phases) were studied by Wojciechowski [22,23]. The term auxetic in the scientific literature was introduced by Evans [24]. The re-entrant hexagonal honeycomb structure is one of the most well-known open-cell auxetic structures [42]. In several studies [43–46], the effect of relative density and re-entrant angle variations on mechanical properties such as Poisson’s ratio and elastic modulus of typical 2D re-entrant structure in the elastic and plastic range have been analyzed for predicting the behavior of the structure. To improve the mechanical properties such as strength and auxeticity of the re-entrant structures and for answering the new requirements in the industry, some researchers have introduced and built novel 3D re-entrant structures inspired by typical 2D re-entrant unit cells and have established analytical and numerical solutions for them [47–50].

The unit cell presented by Yang et al. in 2015 [50] (Figure1a) is one of the successful 3D auxetic structures, which has been solved analytically in two directions and evaluated by experimental and numerical results. In another study, Wang et al. (2016) [51] proposed an interlocking assembly manufacturing technique for fabricating the re-entrant lattice structure proposed by Yang et al. (2015) [50] but with a shifted unit cell (Figure 1b), which showed great advantages over additive manufacturing technique. Chen et al. (2017) and Xue et al. (2020) [52,53] applied some modifications to the noted 3D re-entrant auxetic structure by adding some struts to enhance the mechanical properties of the lattice structure, and in particular, to increase the stiffness of this auxetic structure (Figure1c,d). Although the 3D reentrant structures studied in the noted works are successful auxetic structures for many applications, they still lack some geometrical characteristics, which could raise problems in many applications. First of all, even though the noted 3D re-entrant unit cells are symmetrical in the lateral directions, but their geometry is different in the vertical (i.e., loading) direction. Therefore, they exhibit dissimilar mechanical properties in the three main orthogonal directions, which means that they are not truly 3D auxetic structures. Second, the struts at the edge of the noted unit cells are shared by adjacent unit cells in the lattice structure. Since the auxetic structures are useful in many applications (such as biomedical implants [54,55], sandwich panels [56], etc.) that require graded micro-structures, the noted shared struts cause huge complexities and difficulties in constructing truly graded lattice structures. Hence, there remains a gap to propose an ideal unit cell that could overcome these deficiencies of typical 3D re-entrant structure.

In this study, a specific type of mechanical metamaterial, namely, an idealized 3D
re-entrant structure [41,57] constructed of three strut types, one type loaded purely axially and
two types loaded both flexurally and axially, which are inclined and are spatially defined by
*angles θ and ϕ (see Figure*2), is studied to obtain analytical relationships for its mechanical
properties. Analytical solutions based on two well-known beam theories namely Euler–
Bernoulli and Timoshenko theories are derived. Moreover, two numerical methods one
based on volumetric elements and one based on beam elements are implemented for
validating the results. A definition for strut effective length has been presented in order
to simulate what the struts experience in real-life conditions, and analytical results have
been presented based on the effective length. Moreover, a lightened auxetic unit cell
extracted from the general re-entrant unit cell (presented in Figure2) is introduced and

its mechanical properties are compared to those of the ideal re-entrant structure. Several specimens have also been additively manufactured and tested under compressive loading conditions. Finally, the results of the derived analytical and constructed numerical models and the manufactured specimens are compared to one another.

* Materials 2021, 14, x FOR PEER REVIEW * 3 of 36

**(a) ** **(b) **

**(c) ** **(d) **

**Figure 1. Review of 3D re-entrant unit cells presented by (a) Li Yang et al. (2015) [50], (b) Xin-Tao **

**Wang et al. (2016) [51], (c) Yu Chen et al. (2017) [52], and (d) Yingying Xue et al. (2020) [53]. **
In this study, a specific type of mechanical metamaterial, namely, an idealized 3D
re-entrant structure [41,57] constructed of three strut types, one type loaded purely axially
and two types loaded both flexurally and axially, which are inclined and are spatially
defined by angles 𝜃 and 𝜑 (see Figure 2), is studied to obtain analytical relationships for
its mechanical properties. Analytical solutions based on two well-known beam theories
namely Euler–Bernoulli and Timoshenko theories are derived. Moreover, two numerical
methods one based on volumetric elements and one based on beam elements are
imple-mented for validating the results. A definition for strut effective length has been presented
**Figure 1.Review of 3D re-entrant unit cells presented by (a) Li Yang et al. (2015) [**50**], (b) Xin-Tao**
Wang et al. (2016) [51**], (c) Yu Chen et al. (2017) [**52**], and (d) Yingying Xue et al. (2020) [**53].

**Materials 2021, 14, 993** 4 of 36

* Materials 2021, 14, x FOR PEER REVIEW * 4 of 36

in order to simulate what the struts experience in real-life conditions, and analytical re-sults have been presented based on the effective length. Moreover, a lightened auxetic unit cell extracted from the general re-entrant unit cell (presented in Figure 2) is intro-duced and its mechanical properties are compared to those of the ideal re-entrant struc-ture. Several specimens have also been additively manufactured and tested under com-pressive loading conditions. Finally, the results of the derived analytical and constructed numerical models and the manufactured specimens are compared to one another.

**(a) **

**(b) **

**Type I**
**Type II**
**Type III**

**Figure 2.(a) An idealized 3D re-entrant unit cell and its strut types, (b) degrees of freedom (DOFs) of**
the unit cell. The double arrows represent the rotational degrees of freedom. More illustrations of the
unit cell, its dimensions, and boundary conditions can be found in Figures S1–S5.

**2. Materials and Methods**

2.1. Analytical Solution 2.1.1. Relative Density

Each re-entrant unit cell (Figure2a and Figure S1) consists of three types of struts with lengths l1, l2, l3and cross-sectional areas A1, A2, A3. The unit cell is fully defined with two

*unique angles θ and ϕ, the Type-I strut length, and the main cube size (the main cube is the*
hypothetical cube formed by connecting vertices Diwhere i=*1 to 8). Angle θ is defined*

*as the angle between Type-II strut and the face diagonals of the main cube, and angle ϕ is*
defined as the angle between a Type-III strut and the corresponding side of the main cube
(Figure2b). Each re-entrant unit cell with mentioned strut lengths (l1, l2, l3)and

*character-istic angles (θ, ϕ) occupies a cubic volume with side length of 2*(l1+l3*cos ϕ*−l2*sin θ*)and

hence the volume of Vtotal=8(l1+l3*cos ϕ*−l2*sin θ*)3. Because the unit cell is made up of

six struts of Type I, 24 struts of Type II, and 24 struts of Type III, the volume occupied by
all struts inside the unit cell is Vstrut=*6πr*21l1+*24πr*22l2+*24πr*32l3. Therefore, according to

*the basic definition of relative density µ*= Vstrut

Vtotal, the relative density of a re-entrant unit
cell is given by
*µ*= 6A1l1+24A2l2+24A3l3
Lunitcell3
= *3π r*
2
1l1+4r22l2+4r23l3
4(l1+l3*cos ϕ*−l2*sin θ*)3
(1)
2.1.2. Stiffness Matrix

In this subsection, analytical relationships for mechanical properties of the 3D
re-entrant unit cell such as elastic modulus, Poisson’s ratio, and yield stress are derived as
functions of elastic properties of the bulk material (Es, Gs*, σ*ys, and vs) and the geometrical

dimensions of the unit cell. The re-entrant unit cell has symmetry with respect to its major planes (see Figure S2). Therefore, studying 1/8 of the unit cell is sufficient for obtaining the mechanical properties of the unit cell and, hence, the corresponding lattice structure. Due to the intrinsic symmetries in the geometry of the re-entrant unit cell and the applied boundary conditions on the unit cell, seven unique group of vertices can be recognized, which are denoted by letters A, B, C, D, E, F, and G, as shown in Figure2a. For the sake of brevity and as the vertices named by similar letters demonstrate identical behaviors, in many cases, instead of referring to a vertex as Xi, we refer to it as X (X representing A, B,

C, D, E, F, and G). For instance, in many cases, we use the name E instead of E1.

If the origin of the coordinate system is considered to be located in the midst of the unit cell, each re-entrant unit cell has four vertical (XY, YZ, and two bisectors of XY and YZ) and one horizontal (XZ) symmetry planes (as shown in Figure S2). All the vertices located in the symmetry planes are only allowed to translate and rotate in their corresponding planes. Vertices Aiand Bi (for i = 1, 2) lie in all of the four vertical symmetry planes, so

they are only allowed to translate in the Y direction, and they are constrained rotationally. Therefore, they create two degrees of freedom (DOFs) q8and q7at vertices Ai and Bi,

respectively. Vertices Ci(for i=1 to 8) are located in one of the vertical symmetry planes

(XY or YZ), and hence they are only allowed to translate horizontally and vertically and rotate in their corresponding planes, which results in three other DOFs (q3, q4, q11). Each

vertex Di(for i=1 to 8) is located in a single vertical symmetry plane (one of two bisectors

of YZ and YX), and therefore, it is only allowed to translate horizontally and vertically and rotate in the planes it is located in, which leads to three other DOFs (q5, q6, q10). Vertices

Ei and Fi(for i = 1 to 4) are located in one of two vertical symmetry planes (XY or YZ)

and the horizontal symmetry plane XZ, so they are only allowed to translate in the X or Z directions without any rotations. This creates two other DOFs q2and q1at vertices E and F,

respectively. Vertices Giare located in the horizontal symmetry plane XZ and in one of the

vertical bisector symmetry planes (bisectors of XY and YZ). Therefore, these points cannot rotate in any directions and are only allowed to translate horizontally in the bisector of the noted planes, which leads to the final DOF q9. Overall, the system has a total number of

11 DOFs (Figure2b).

In this study, two well-known elastic beam theories, namely, Euler–Bernoulli and Timoshenko beam theories, have been implemented for analytical analysis of the re-entrant unit cell. As the beam theories and material models used for the analytical analysis are linear, the overall deformation of each DOF in the system can be considered as the superposition of separate deformations caused by applying individual loads at each DOF.

**Materials 2021, 14, 993** 6 of 36

Therefore, the superposition principle could be implemented for obtaining the system of equations of the unit cell. In this approach, each DOF displaces autonomously from other DOFs, and when a DOF is displaced, the other DOFs are kept fixed. By solving the equilibrium equations for the vertices of the unit cell, the resultant forces are obtained. By considering this method, the system of equilibrium equations for the structure could be written as{Q} = [K]{q}. In this equation,{Q}is the force vector comprising the external forces acting on the DOFs,[K]is the stiffness matrix of the system, and the{q}is the displacement vector.

Because the derivation of the stiffness matrix elements is based on beam theories, the general deformation of a cantilever beam (Figure3) can be considered as the resultant of four distinct deformations at the free end of the beam, which are as follows:

(a) a lateral displacement without any rotation, v;

(b) *a flexural rotation without any lateral displacement, θ;*
(c) a longitudinal elongation or contraction, u;

(d) *an axial twist, ϕ.*

* Materials 2021, 14, x FOR PEER REVIEW * 6 of 36

translate in the X or Z directions without any rotations. This creates two other DOFs 𝑞 and 𝑞 at vertices E and F, respectively. Vertices 𝐺 are located in the horizontal symmetry plane XZ and in one of the vertical bisector symmetry planes (bisectors of XY and YZ). Therefore, these points cannot rotate in any directions and are only allowed to translate horizontally in the bisector of the noted planes, which leads to the final DOF 𝑞 . Overall, the system has a total number of 11 DOFs (Figure 2b).

In this study, two well-known elastic beam theories, namely, Euler–Bernoulli and Timoshenko beam theories, have been implemented for analytical analysis of the re-en-trant unit cell. As the beam theories and material models used for the analytical analysis are linear, the overall deformation of each DOF in the system can be considered as the superposition of separate deformations caused by applying individual loads at each DOF. Therefore, the superposition principle could be implemented for obtaining the system of equations of the unit cell. In this approach, each DOF displaces autonomously from other DOFs, and when a DOF is displaced, the other DOFs are kept fixed. By solving the equi-librium equations for the vertices of the unit cell, the resultant forces are obtained. By considering this method, the system of equilibrium equations for the structure could be written as {𝑄} = [𝐾]{𝑞}. In this equation, {𝑄} is the force vector comprising the external forces acting on the DOFs, [𝐾] is the stiffness matrix of the system, and the {𝑞} is the dis-placement vector.

Because the derivation of the stiffness matrix elements is based on beam theories, the general deformation of a cantilever beam (Figure 3) can be considered as the resultant of four distinct deformations at the free end of the beam, which are as follows:

(a) a lateral displacement without any rotation, 𝑣;

(b) a flexural rotation without any lateral displacement, 𝜃; (c) a longitudinal elongation or contraction, 𝑢;

(d) an axial twist, 𝜑.

**Figure 3. General deformation of a cantilever beam with axial and lateral displacements in **

*addi-tion to flexural and torsional rotaaddi-tions in its free end. *

The corresponding forces and moments required to create each of the pure above-mentioned deformations are demonstrated in Figure 4 for the Euler–Bernoulli and Timo-shenko beam theories. Due to frequent repetition of some terms demonstrated in Figure 4 throughout the whole manuscript, the terms 𝑆 , 𝑊 , 𝑇 , 𝑉 , and 𝑈 are used, which are dif-ferent for Euler–Bernoulli and Timoshenko beam theories and are listed in Table 1.

**Figure 3.**General deformation of a cantilever beam with axial and lateral displacements in addition
to flexural and torsional rotations in its free end.

The corresponding forces and moments required to create each of the pure above-mentioned deformations are demonstrated in Figure4for the Euler–Bernoulli and Timo-shenko beam theories. Due to frequent repetition of some terms demonstrated in Figure4

throughout the whole manuscript, the terms Si, Wi, Ti, Vi, and Ui are used, which are

different for Euler–Bernoulli and Timoshenko beam theories and are listed in Table1.

**Table 1.**Parameters defined for summarizing the relationships for Euler–Bernoulli and Timoshenko
beam theories.

**Term** **Euler-Bernoulli Theory** **Timoshenko Theory**

Si Ai_{li}Es Ai_{li}Es
Wi Gs_{li}Ji Gs_{li}Ji
Ti 12EsIi_{l}3
i
1
l3_{i}
12Es Ii+*κ Ai Gs*li
Vi 6Es_{l}2Ii
i
1
l2_{i}
6Es Ii+
2
*κ Ai Gs*
Ui 4Es_{l}Ii
2Es Ii
*κ Ai Gs l*+
2li
3
l2_{i}
6Es Ii+
2
*κ Ai Gs*

**(a) **

**(b) **

**(c) **

**(d) **

**Figure 4. Forces and moments required to cause (a) lateral displacement 𝛿 with no rotation, (b) **

**flexural rotation 𝜃 with no lateral displacement, (c) pure axial extension, and (d) pure twist at the **
free end of a beam [58].

**Table 1. Parameters defined for summarizing the relationships for Euler–Bernoulli and **

Timo-shenko beam theories.

**Term ** **Euler-Bernoulli **

**Theory ** **Timoshenko Theory **

𝑆 𝐴 𝐸_{𝑙} 𝐴 𝐸_{𝑙}
𝑊 𝐺 𝐽_{𝑙} 𝐺 𝐽_{𝑙}
𝑇 12𝐸 𝐼_{𝑙}
1
𝑙
12𝐸 𝐼 +𝜅𝐴 𝐺𝑙

**Figure 4.****Forces and moments required to cause (a) lateral displacement δ with no rotation, (b) flexural rotation θ with no****lateral displacement, (c) pure axial extension, and (d) pure twist at the free end of a beam [**58].

To explain the general procedure for deriving the stiffness matrix elements, we could
consider a strut PQ with an arbitrary orientation with respect to the global X, Y, and Z
**coordinate system (aligned with a unit vector u**PQ), which is deformed by a specific DOF
**q**_{i}at its free end. The schematic representation of such a strut and its deformation due to
the DOF is illustrated in Figure5**. As shown in the figure, DOF q**_{i}causes a longitudinal
and a transverse deformation in the strut PQ. The vector of longitudinal deformation
**of strut PQ can be obtained by projecting the vector q**_{i}on the strut PQ unit vector, i.e.,

**q**_{i}·**u**PQ**u**PQ. Moreover, the vector of transverse deformation of strut PQ can be obtained

**as q**_{i}− **q**_{i}·**u**PQ**u**PQ. By multiplying the longitudinal deformation vector of strut PQ by

the resultant force value of PQ (i.e., Si), the resultant longitudinal force vector for strut

PQ can be obtained as **q**_{i}·**u**PQ**u**PQSi, and by multiplying the transverse deformation

vector of strut PQ by the resultant transverse force value of PQ (i.e., Ti), the resultant

**Materials 2021, 14, 993** 8 of 36

moment vector, created by the transverse deformation of strut PQ can be found by the
**cross-product of the unit vector of PQ (i.e., u**PQ) and the resultant moment vector of the beam

**(i.e., q**_{i}− **q**_{i}·**u**PQ**u**PQVi), which yields− **u**PQ× **q**i− **q**i·**u**PQ**u**PQVi. The values of

Si, Ti, and Vifor Timoshenko and Euler–Bernoulli beam theories are listed in Table1. It is

worth noting that the procedure of obtaining the forces and moments for a lateral rotational DOF is very similar to the above-mentioned procedure, and it could be easily performed by replacing the terms Si, Ti, and Viwith the terms Wi, Vi, and Ui, respectively.

* Materials 2021, 14, x FOR PEER REVIEW * 8 of 36

𝑉 6𝐸 𝐼_{𝑙}
1
𝑙
6𝐸 𝐼 +𝜅𝐴 𝐺2
𝑈 4𝐸 𝐼
𝑙
2𝐸 𝐼
𝜅𝐴 𝐺 𝑙 +2𝑙3
𝑙
6𝐸 𝐼 +𝜅𝐴 𝐺2

To explain the general procedure for deriving the stiffness matrix elements, we could
consider a strut PQ with an arbitrary orientation with respect to the global X, Y, and Z
coordinate system (aligned with a unit vector 𝒖 ), which is deformed by a specific DOF
**𝒒 at its free end. The schematic representation of such a strut and its deformation due to **
the DOF is illustrated in Figure 5. As shown in the figure, DOF 𝒒 causes a longitudinal
and a transverse deformation in the strut PQ. The vector of longitudinal deformation of
**strut PQ can be obtained by projecting the vector 𝒒 on the strut PQ unit vector, i.e., **
𝒒 · 𝒖 𝒖 . Moreover, the vector of transverse deformation of strut PQ can be obtained
as 𝒒 − 𝒒 · 𝒖 𝒖 . By multiplying the longitudinal deformation vector of strut PQ by
the resultant force value of PQ (i.e., 𝑆 ), the resultant longitudinal force vector for strut PQ
can be obtained as 𝒒 . 𝒖 𝒖 𝑆 , and by multiplying the transverse deformation
vec-tor of strut PQ by the resultant transverse force value of PQ (i.e., 𝑇 ), the resultant
trans-verse force vector for this strut can be obtained as 𝒒 − 𝒒 · 𝒖 𝒖 𝑇 . The reaction
mo-ment vector, created by the transverse deformation of strut PQ can be found by the
**cross-product of the unit vector of PQ (i.e., 𝒖 ) and the resultant moment vector of the beam **
(i.e., 𝒒 − 𝒒 · 𝒖 𝒖 𝑉 ), which yields − 𝒖 × 𝒒 − 𝒒 · 𝒖 𝒖 𝑉 . The values of
𝑆 , 𝑇 , and 𝑉 for Timoshenko and Euler–Bernoulli beam theories are listed in Table 1. It is
worth noting that the procedure of obtaining the forces and moments for a lateral
rota-tional DOF is very similar to the above-mentioned procedure, and it could be easily
per-formed by replacing the terms 𝑆 , 𝑇 , and 𝑉 with the terms 𝑊 , 𝑉 , and 𝑈 , respectively.

In the following, the detailed procedure of derivation of the stiffness matrix elements for three distinct DOFs (𝑞 , 𝑞 , and 𝑞 ) are presented. The derivation procedure of other DOFs is similar to the ones presented in the paper, but they are provided in Section S.1.2 and Figure S6.

**(a) **

* Materials 2021, 14, x FOR PEER REVIEW * 9 of 36

**(b) **

**Figure 5. General deformation of a strut due to 𝑞 = 1 (a) magnitude of deformations and (b) **

**re-sultant forces and moments. **

(a) First DOF: 𝑞 = 1

Here, the elements of the first column of the stiffness matrix are derived by applying
the unit displacement 𝑞 = 1 and by keeping all the other DOFs fixed (i.e., = 0). This
de-formation type displaces point 𝐹 horizontally in the Z direction. This dede-formation only
causes elongation in strut EF and it does not affect the other struts. The vector of
elonga-tion of strut EF can be obtained by projecting the vector 𝒒 on strut EF, i.e., 𝑞⃗. ⃗_{⃗} ⃗_{⃗}
or in a simpler notation 𝒒 . 𝒖 𝒖 **, where 𝒒 is the unit vector parallel to the first **
**DOF, and 𝒖** is the unit vector parallel to strut 𝐸 𝐹 . The same system of notation will
be used in the rest of the document. By multiplying the elongation vector of strut EF by
the resultant force parameter of strut EF (i.e., 𝑆 ), the resultant force vector can be obtained
as 𝒒 . 𝒖 𝒖 𝑆 .

The equilibrium of forces at point 𝐹 in the 𝑞 direction, i.e., the Z direction, provides the 𝐾 element of the stiffness matrix (Figure 6), which is calculated as

𝐹, = 0 → 𝑄_{4} − 𝒒 · 𝒒 · 𝒖 𝒖 𝑆 = 0 → 𝐾 = 𝑄 = 4𝑆 (2)
It must be noted that the forces demonstrated in Figure 6 are the only forces that must
act on the beam in order for it to deform in the way it is shown. The force the beam applies
at each vertex is in the opposite direction of what is shown in Figure 6. The same holds
true for all the next derivations. The equilibrium of forces at point 𝐸 in the 𝑞 direction
(i.e., in the Z direction) provides the 𝐾 element of the stiffness matrix, which is calculated
as

𝐹, = 0 → 𝑄_{4} + 𝒒 · 𝒒 · 𝒖 𝒖 𝑆 = 0 → 𝐾 = 𝑄 = −4𝑆 (3)
Because the displacement of DOF 𝒒 does not have any effect on other DOFs
(𝒒 , 𝒒 , 𝒒 , 𝒒 , 𝒒 , 𝒒 , 𝒒 , 𝒒 , 𝒒 ), the remaining elements of the first column of the stiffness
matrix are zero.

**Figure 5.**General deformation of a strut due to qi=**1 (a) magnitude of deformations and (b) resultant forces and moments.**

In the following, the detailed procedure of derivation of the stiffness matrix elements for three distinct DOFs (q1, q2, and q10) are presented. The derivation procedure of other

DOFs is similar to the ones presented in the paper, but they are provided in Section S.1.2 and Figure S6.

(a) First DOF: q1=1

Here, the elements of the first column of the stiffness matrix are derived by applying the unit displacement q1 = 1 and by keeping all the other DOFs fixed (i.e., = 0). This

deformation type displaces point F1horizontally in the Z direction. This deformation only

**of strut EF can be obtained by projecting the vector q**_{1}on strut EF, i.e.,
→
q1·
→
E1F1
→
E1F1
→
E1F1
→
E1F1
or
**in a simpler notation q**_{1}·**u**E1F1**u**E1F1**, where q**1is the unit vector parallel to the first DOF,

**and u**E1F1 is the unit vector parallel to strut E1F1. The same system of notation will be
used in the rest of the document. By multiplying the elongation vector of strut EF by the
resultant force parameter of strut EF (i.e., S1), the resultant force vector can be obtained as

**q**_{1}·**u**E1F1**u**E1F1S1.

The equilibrium of forces at point F1in the q1direction, i.e., the Z direction, provides

the K11element of the stiffness matrix (Figure6), which is calculated as

### ∑

Fz,F1 =0 → Q14 −**q**1· **q**1·**u**E1F1**u**E1F1S1=0 →K11=Q1=4S1 (2)

* Materials 2021, 14, x FOR PEER REVIEW * 10 of 36

**Figure 6. Deformation of strut EF due to 𝑞 = 1. **

(b) Second DOF: 𝑞 = 1

In this subsection, the elements of the second column of the stiffness matrix are
de-rived. Therefore, we set 𝑞 = 1, and the other DOFs are set to zero. This deformation type
displaces point E horizontally in the Z direction, which causes strut EF to have a pure
contraction and strut ED to have contraction accompanied by transverse displacement.
**The vector of contraction of strut EF can be obtained by projecting vector 𝒒 on strut EF, **
i.e., 𝒒 . 𝒖 𝒖 . The vector of contraction of strut ED can be obtained by projecting
vector 𝒒𝟐** on strut ED, i.e., 𝒒 . 𝒖** 𝒖 , and the vector of transverse displacement of
vertex E of strut ED can be calculated as 𝒒 − 𝒒 . 𝒖 𝒖 .

By multiplying the contraction vector of strut EF by the resultant force parameter of strut EF (i.e., 𝑆 ), the resultant force vector of strut EF can be obtained as

𝒒 . 𝒖 𝒖 𝑆 . Moreover, by multiplying the elongation vector of strut ED by the resultant force parameter of strut ED (i.e., 𝑆 ), the resultant force vector can be obtained as 𝒒 . 𝒖 𝒖 𝑆 . Finally, by multiplying the transverse deformation vector of strut ED by the resultant transverse force parameter of strut ED (i.e., 𝑇 ), the resultant trans-verse force vector of this strut can be obtained as 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 . It is worth noting that the resultant forces obtained for deformation of struts ED at point E must be multiplied by four because there are four similar struts ED connected to point E. The equi-librium of forces at point E in the 𝑞 direction (i.e., the Z direction), Figure 7b, provides the element 𝐾 of the stiffness matrix as follows:

𝐹, = 0 →
𝑄
4 − 𝒒 . 𝒒 . 𝒖 𝒖 𝑆 + 4 𝒒 . 𝒒 . 𝒖 𝒖 𝑆 − 4 𝒒 . 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 = 0
→ 𝐾 = 𝑄 = 4(𝑆 + 4 sin 𝜃 𝑆 + 4 cos 𝜃 𝑇 )
(4)
**(a) **

**Figure 6.**Deformation of strut EF due to q1=1.

It must be noted that the forces demonstrated in Figure6are the only forces that must act on the beam in order for it to deform in the way it is shown. The force the beam applies at each vertex is in the opposite direction of what is shown in Figure6. The same holds true for all the next derivations. The equilibrium of forces at point E1in the q2direction (i.e., in

the Z direction) provides the K12element of the stiffness matrix, which is calculated as

### ∑

Fz,E1 =0 → Q24 +**q**2· **q**1·**u**E1F1**u**E1F1S1=0 →K12 =Q2= −4S1 (3)
**Because the displacement of DOF q**_{1} does not have any effect on other DOFs
**(q**_{3}**, q**_{4}**, q**_{5}**, q**_{6}**, q**_{7}**, q**_{8}**, q**_{9}**, q**_{10}**, q**_{11}), the remaining elements of the first column of the
stiffness matrix are zero.

(b) Second DOF: q2=1

In this subsection, the elements of the second column of the stiffness matrix are derived. Therefore, we set q2=1, and the other DOFs are set to zero. This deformation

type displaces point E horizontally in the Z direction, which causes strut EF to have a pure
contraction and strut ED to have contraction accompanied by transverse displacement.
**The vector of contraction of strut EF can be obtained by projecting vector q**_{2}on strut EF, i.e.,

**q**_{2}·**u**E1F1**u**E1F1. The vector of contraction of strut ED can be obtained by projecting vector

**q**_{2}**on strut ED, i.e., q**_{2}·**u**E_{1}D_{1}**u**E_{1}D_{1}, and the vector of transverse displacement of vertex E

**of strut ED can be calculated as q**_{2}− **q**_{2}·**u**E1D1**u**E1D1.

By multiplying the contraction vector of strut EF by the resultant force parameter of
strut EF (i.e., S1), the resultant force vector of strut EF can be obtained as **q**2·**u**E1F1**u**E1F1S1.
Moreover, by multiplying the elongation vector of strut ED by the resultant force parameter
of strut ED (i.e., S2), the resultant force vector can be obtained as **q**2·**u**E1D1**u**E1D1S2.
Finally, by multiplying the transverse deformation vector of strut ED by the resultant
transverse force parameter of strut ED (i.e., T2), the resultant transverse force vector of

**this strut can be obtained as q**_{2}− **q**_{2}·**u**E1D1**u**E1D1T2. It is worth noting that the resultant
forces obtained for deformation of struts ED at point E must be multiplied by four because
there are four similar struts ED connected to point E. The equilibrium of forces at point E
in the q2direction (i.e., the Z direction), Figure7b, provides the element K22of the stiffness

**Materials 2021, 14, 993** 10 of 36

∑ Fz,E1=0 → Q24 −**q**2·((**q**2·**u**E1F1)**u**E1F1)S1+4(**q**2·((**q**2·**u**E1D1)**u**E1D1)S2) −4(**q**2·(**q**2− (**q**2·**u**E1D1)**u**E1D1)T2) =0

→K22=Q2=4 S1+4 sin2*θS*2+4 cos2*θT*2

(4)

* Materials 2021, 14, x FOR PEER REVIEW * 10 of 36

**Figure 6. Deformation of strut EF due to 𝑞 = 1. **

(b) Second DOF: 𝑞 = 1

In this subsection, the elements of the second column of the stiffness matrix are
de-rived. Therefore, we set 𝑞 = 1, and the other DOFs are set to zero. This deformation type
displaces point E horizontally in the Z direction, which causes strut EF to have a pure
contraction and strut ED to have contraction accompanied by transverse displacement.
**The vector of contraction of strut EF can be obtained by projecting vector 𝒒 on strut EF, **
i.e., 𝒒 . 𝒖 𝒖 . The vector of contraction of strut ED can be obtained by projecting
vector 𝒒𝟐** on strut ED, i.e., 𝒒 . 𝒖** 𝒖 , and the vector of transverse displacement of
vertex E of strut ED can be calculated as 𝒒 − 𝒒 . 𝒖 𝒖 .

By multiplying the contraction vector of strut EF by the resultant force parameter of strut EF (i.e., 𝑆 ), the resultant force vector of strut EF can be obtained as

𝒒 . 𝒖 𝒖 𝑆 . Moreover, by multiplying the elongation vector of strut ED by the resultant force parameter of strut ED (i.e., 𝑆 ), the resultant force vector can be obtained as 𝒒 . 𝒖 𝒖 𝑆 . Finally, by multiplying the transverse deformation vector of strut ED by the resultant transverse force parameter of strut ED (i.e., 𝑇 ), the resultant trans-verse force vector of this strut can be obtained as 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 . It is worth noting that the resultant forces obtained for deformation of struts ED at point E must be multiplied by four because there are four similar struts ED connected to point E. The equi-librium of forces at point E in the 𝑞 direction (i.e., the Z direction), Figure 7b, provides the element 𝐾 of the stiffness matrix as follows:

𝐹, = 0 →
𝑄
4 − 𝒒 . 𝒒 . 𝒖 𝒖 𝑆 + 4 𝒒 . 𝒒 . 𝒖 𝒖 𝑆 − 4 𝒒 . 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 = 0
→ 𝐾 = 𝑄 = 4(𝑆 + 4 sin 𝜃 𝑆 + 4 cos 𝜃 𝑇 )
(4)
**(a) **

* Materials 2021, 14, x FOR PEER REVIEW * 11 of 36

**(b) **

**Figure 7. Deformation and loads applied on struts (a) EF and (b) ED due to 𝑞 = 1. **

The presence of reaction forces and moments at point D due to 𝒒 leads to non-zero values of 𝐾 , 𝐾 , and 𝐾 . By projecting the resultant contraction force vector

𝒒 . 𝒖 𝒖 𝑆 and the transverse deformation force vector 𝒒 −
𝒒 . 𝒖 𝒖 **𝑇 of strut ED in the 𝒒 and 𝒒 directions, and solving the equilibrium of **
forces at point D in these two directions, the elements 𝐾 and 𝐾 of the stiffness matrix
could be obtained. It is important to note that the force vectors at point D have been
mul-tiplied by two (as two ED struts are connected to point D):

𝐹, = 0 →
𝑄
8 + 2𝒒 . 𝒒 . 𝒖 𝒖 𝑆 + 2𝒒 . 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 = 0
→ 𝐾 = 𝑄 = 4√2 sin 2𝜃 (𝑇 − 𝑆 )
(5)
𝐹 , = 0 → 𝑄_{8} + 2𝒒 . 𝒒 . 𝒖 𝒖 𝑆 + 2𝒒 . 𝒒 − 𝒒 . 𝒖 𝒖 𝑇 = 0
→ 𝐾 = 𝑄 = 4 sin 2𝜃 (𝑇 − 𝑆 ) − 8√2 sin 𝜃 𝑆 − 8√2 cos 𝜃 𝑇

(6)

To obtain the element 𝐾 of the stiffness matrix, the equilibrium of moments in the
𝑞 direction at point D must be considered. The reaction moment vector, created by
trans-verse deformation of point E of strut ED can be obtained by the cross-product of unit
vec-tor of strut ED, 𝒖 , and the resultant moment vector of the beam at point D,
i.e., 𝒒 − 𝒒 . 𝒖 𝒖 𝑉 . This vector must be multiplied by two in the equilibrium
equation as two struts ED are connected to point D. Finally, by solving the equilibrium of
moments in the 𝑞 direction, the element 𝐾 of the stiffness matrix could be derived:
𝑀 , = 0 → 𝑄_{8} + 2𝒒 · 𝒖 × 𝒒 − 𝒒 · 𝒖 𝒖 𝑉 = 0 → 𝐾 = 𝑄 = −8 cos 𝜃 𝑉 (7)

(c) The 10th DOF: 𝑞 = 1

This DOF is a complex deformation in the structure because it applies rotation at vertex D, which is connected to six struts (2 × DC, 2 × DE, DG, and DB). By projecting

**Figure 7.Deformation and loads applied on struts (a) EF and (b) ED due to q**2=1.

**The presence of reaction forces and moments at point D due to q**_{2} leads to
non-zero values of K25, K26, and K210. By projecting the resultant contraction force vector
**q**_{2}·**u**E1D1**u**E1D1S2**and the transverse deformation force vector q**2− q2·**u**E1D1**u**E1D1T2
**of strut ED in the q**_{5}**and q**_{6}directions, and solving the equilibrium of forces at point D in
these two directions, the elements K25and K26of the stiffness matrix could be obtained. It

is important to note that the force vectors at point D have been multiplied by two (as two ED struts are connected to point D):

∑ Fy,D1 =0 →
Q5
8 +**2q**5· **q**2·**u**E1D1**u**E1D1S2+**2q**5· **q**2− **q**2·**u**E1D1**u**E1D1T2=0
→K25=Q5=4
√
*2 sin 2θ*(T2−S2)
(5)

∑ F**q**_{6},D1 =0 →
Q6
8 +**2q**6· **q**2·**u**E1D1**u**E1D1S2+**2q**6· **q**2− **q**2·**u**E1D1**u**E1D1T2=0
→K26=Q6=*4 sin 2θ*(T2−S2) −8
√
2 sin2*θS*2−8
√
2 cos2* _{θT}*
2
(6)
To obtain the element K210 of the stiffness matrix, the equilibrium of moments in

the q10direction at point D must be considered. The reaction moment vector, created by

transverse deformation of point E of strut ED can be obtained by the cross-product of
**unit vector of strut ED, u**E1D1, and the resultant moment vector of the beam at point D,
**i.e., q**_{2}− **q**_{2}·**u**E_{1}D_{1}**u**E_{1}D_{1}V2. This vector must be multiplied by two in the equilibrium

equation as two struts ED are connected to point D. Finally, by solving the equilibrium of moments in the q10direction, the element K210 of the stiffness matrix could be derived:

### ∑

Mq10,D1 =0 → Q108 +**2q**10· **u**E1D1× **q**2− **q**2·**u**E1D1**u**E1D1V2=0 →K210=Q10 = −*8 cos θV*2 (7)
(c) The 10th DOF: q10=1

This DOF is a complex deformation in the structure because it applies rotation at
vertex D, which is connected to six struts (2 × DC, 2 × DE, DG, and DB). By
**pro-jecting vector q**_{10} on the noted struts, the torsion applied to each of the struts can be
**found (q**_{10}·uC1D1**, q**10·**u**E1D1**, q**10·**u**B1D1**, q**10·**u**G1D1). Afterward, by multiplying the
tor-sional parameter of each strut (W2 and W3) by the projected twist, the torque vectors

could be obtained as **q**_{10}·**u**C1D1**u**C1D1W3, **q**10·**u**E1D1**u**E1D1W2, **q**10·**u**B1D1**u**B1D1W2,
and **q**_{10}·**u**G1D1**u**G1D1W3. The extent of flexural rotation of struts DC, DE, DG, and
**DB can be obtained by subtracting the projected twist vector from vector q**_{10}, which
**yields q**_{10}− **q**_{10}·**u**C_{1}D_{1}**u**C_{1}D_{1}**, q**10− **q**10·**u**E1D1**u**E1D1**, q**10− **q**10·**u**B1D1**u**B1D1**, and q**10−
**q**_{10}·**u**G1D1**u**G1D1, respectively. Afterward, by multiplying the resultant bending parameter
of each strut (i.e., U2and U3) to the noted terms, the lateral force vectors could be

calcu-lated. It is worth noting that the terms related to struts CD and ED must be multiplied
by two because two of such struts are connected to point D. Finally, by projecting all the
**resultant axial and lateral moments in the q**_{10}direction and writing the equation of moment
equilibrium in this direction, the element K1010can be found:

∑ M**q**_{10},D1 =0 →
Q10
8 −**2q**10· **q**10·**u**C1D1**u**C1D1W3−**2q**10· **q**10− **q**10·**u**C1D1**u**C1D1U3−**2q**10
· **q**_{10}·**u**E1D1**u**E1D1W2−**2q**10· **q**10− **q**10·**u**E1D1**u**E1D1U2−**q**10· **q**10·**u**B1D1**u**B1D1W2−**q**10
· **q**_{10}− **q**_{10}·**u**B1D1**u**B1D1U2−**q**10· **q**10·**u**G1D1**u**G1D1W3−**q**10· **q**10− **q**10·**u**G1D1**u**G1D1U3=0
→K1010 =Q10 = 2
3+*cos 2ϕ*−2√*2 sin 2ϕ*W3+2W2
2 sin2*θ*+cos2*θ*−2
√
*2 sin 2θ*

+2√*2 sin 2θU*2−2 cos2*θU*2+

2(5+*cos 2θ*)U2+
9−*cos 2ϕ*+2√*2 sin 2ϕ*U3
(8)

The element K1011could be obtained by solving the equilibrium of moments at vertex

C. By projecting the reaction torsion and bending moment vectors created by the rotation of
**vertex D of strut CD in the q**_{10}direction and solving the equations of moment equilibrium
in the same direction, the element K1011could be calculated as follows:

∑ M**q**_{11},C1 =0 →
Q11
8 −**2q**11· **q**10·**u**C1D1**u**C1D1W3−**2q**11· **q**10− **q**10·**u**C1D1**u**C1D1
U3
2 =0
→K1011=Q11 = −4
2√2 cos2*ϕ*−*sin 2ϕ*
W3+2
*sin 2ϕ*+2√2 sin2*ϕ*
U3
(9)

**Materials 2021, 14, 993** 12 of 36

2.1.3. Stiffness Matrix Derivation

Finally, using the stiffness matrix elements obtained in Section2.1.2 and also by considering the loading condition (Q8=2F), the stiffness matrix and system of equations

can be constructed as 0 0 0 0 0 0 0 2F 0 0 0 = A11 A12 A13 q1 q2 q3 q4 q5 q6 q7 q8 q9 q10 q11 (10)

where F is the external load applied on the unit cell. [A11],[A12], and[A13]are the partial

matrices included in the overall stiffness matrix[K].[A11],[A12], and[A13]have been used

for easier representation of the overall stiffness matrix and are as follows:

A11=
4S1 −4S1 0 0
−4S1 4 S1+4 sin2*θS*2+4 cos2*θT*2
0 0
0 0 8 sin2
*θS*3+4(3+*cos 2ϕ*)T3 8 sin2*ϕ*(S3−T3)
0 0 8 sin2
*ϕ*(S3−T3) 8 sin2*ϕS*3+4(3+*cos 2ϕ*])T3
0 *16 cos ϕ sin θL*3(−S2+T2)
L2 8 sin
2* _{ϕS}*
3+4(3+

*cos 2ϕ*)T3 8 sin2

*ϕ*(S3−T3) 0 −8 √

2(cos ϕ sin θL3(S2−T2)+L2(sin2*θS*2+cos2*θT*2))

L2 4

√

*2 sin ϕ*√*2 cos ϕ*+*sin ϕ*(S3−T3) 4
√

2*sin ϕ*√*2 cos ϕ*+*sin ϕ*S3−

−2+√*2 cos ϕ sin ϕ*+sin2* _{ϕ}*
T3
0 0 0 0
0 0 0 0
0 0 0 0
0 −8√

*2 cos ϕL*3V2 L2 −8 √

*2 cos ϕ*+*sin ϕ*V3 *8 sin ϕV*3

0 0 −8√*2 sin ϕV*3 8
√
*2 sin ϕV*3

A12=
0 0 0 0
*16 cos ϕ sin θL*3(−S2+T2)
L2 −

8√2(*cos ϕ sin θL*3(S2−T2)+L2(sin2* _{θS}*
2+cos2

*2)) L2 0 0 8 sin2*

_{θT}*3+4(3+*

_{ϕS}*cos 2ϕ*)T3

*4 sin ϕ*

*2 cos ϕ*+√

*2 sin ϕ*(S3−T3) 0 0 8 sin2

_{ϕ}_{(}

_{S}3−T3)

*4 sin ϕ*

*2 cos ϕ*+√

*2 sin ϕ*S3−4 −2√2+√2 sin2

_{ϕ}_{+}

*T3 0 0 4 2 sin2*

_{sin 2ϕ}*2+2S3+4 cos 2*

_{θS}*2 3(S2−T2) L2 2 +5T2+*

_{ϕL}*cos 2θT*2+4T3 16√

*2 cos ϕ sin θL*3(S2−T2) L2 + 8√2 cos2

*2 3(S2−T2) L2 2*

_{ϕL}+*4 sin ϕ**4 cos ϕ*+√*2 sin ϕ*(S3−T3) 8 sin2*θS*2+cos2*θT*2 0
16√*2 cos ϕ sin θL*3(S2−T2)
L2 +
8√2 cos2
*ϕL*23(S2−T2)
L2
2

+*4 sin ϕ**4 cos ϕ*+√*2 sin ϕ*(S3−T3) 2

4 sin2_{θS}

2+

5−*cos 2ϕ*+2√*2 sin 2ϕ*S3+*8 cos ϕ sin θL*3

(S2−T2)
L2 +
12 cos2
*ϕL*23(S2−T2)
L2
2
+10T2+*2 cos 2θT*2+7T3+*cos 2ϕT*3−2
√
*2 sin 2ϕT*3
8√*2 cos ϕ sin θL*3(S2−T2)
L2 0
8 sin2* _{θS}*
2+cos2

*θT*2 8 √

*2 cos ϕ sin θL*3(S2−T2) L2 2 S1+4 sin 2

*2+4 cos2*

_{θS}*θT*2 −2S1 0 0 −2S1 2S1

*8 cos ϕ sin ϕ*(−S3+T3) −8 sin2*ϕS*3+cos2*ϕT*3 0 0

−8√2(*sin θL*2+*2 cos ϕL*3)V2
L2 −8
√
*2 cos ϕ*+*2 sin ϕ*V3 8
*sin θ*+*2 cos ϕL*3
L2
V2+
*cos ϕ*+√*2 sin ϕ*V3
−8√*2 cos ϕL*3V2
L2 0
−8√*2 sin ϕV*3 *8 sin ϕV*3 0 0
and
A13=
0 0 0
0 −8
√
*2 cos ϕL*3V2
L2 0
0 −8√*2 cos ϕ + sin ϕ*V3 −8
√
*2 sin ϕV*3
0 *8 sin ϕV*3 8
√
*2 sin ϕV*3
*8 cos ϕ sin ϕ(−S*3+ T3) −8
√
*2(sin θL*2*+2 cos ϕL*3)V2
L2 − 8
√
*2 cos ϕ + 2 sin ϕ*V3 −8
√
*2 sin ϕV*3
−8 sin2_{ϕS}

3+ cos2*ϕT*_{3} 8*sin θ +2 cos ϕL*3

L2
V2+
*cos ϕ +*√*2 sin ϕ*V3
*8 sin ϕV*3
0 −8
√
*2 cos ϕL*3V2
L2 0
0 0 0

8 sin2*ϕS*3+ cos2*ϕT*3 *−8 cos ϕV*3 0

*−8 cos ϕV*3 2((*3+cos 2ϕ−2*
√

*2 sin 2ϕ*)W3L22+4W2(sin θL2*−cos ϕL*3)2*+8 cos ϕ sin θL*2L3U2−4 cos2*ϕL*2_{3}U2+L22(*2(5+cos 2θ)U*2+(*9−cos 2ϕ+2*

√

*2 sin 2ϕ*)U3))

L2 2

*−8 cos ϕ*√*2 cos ϕ − sin ϕ*W3*+ 4 sin ϕ*

*cos ϕ +*√*2 sin ϕ*U3

0 *−8 cos ϕ*√*2 cos ϕ − sin ϕ*W3*+ 4 sin ϕ*

*cos ϕ +*√*2 sin ϕ*U3 16 cos2*ϕW*_{3}+ sin2*ϕU*_{3}

(11)

**Materials 2021, 14, 993** 14 of 36

2.1.4. Elastic Properties Relationships

All the unknown displacements and rotations q1to q11can be obtained as functions of

external force FUCby inverting the final stiffness matrix[K] = [A11] [A12] [A13]

and multiplying it by the force vector. By having the DOF displacements as functions of the applied external force, unit cell elastic mechanical properties such as elastic modulus, Poisson’s ratio, and yield stress can be obtained. The elastic modulus of the unit cell can be calculated according to the basic definition of elastic modulus as follows:

EUC=

FUCLUC

AUC*δ*UC

(12)
where, FUC, LUC, AUC*, δ*UC, and EUCare the applied external load, unit cell length, unit

cell cross-sectional area, unit cell displacement, and elastic modulus of the re-entrant unit
cell, respectively. By considering FUC=*F, δ*UC=2q8, LUC=2(l1+l3*cos ϕ*−l2*sin θ*), and

AUC=LUC2, the elastic modulus of the re-entrant unit cell can be obtained as

EUC=

F

4(l1+l3*cos ϕ*−l2*sin θ*)q8 (13)

Calculation of q8from solving Equation (10) and inserting it in Equation (13) provides

the elastic modulus relationship of the re-entrant unit cell. Because the final relationships
for mechanical properties of the unit cell are very lengthy, the elastic modulus relationship
*for a specific case (θ*=*ϕ*=0◦, r1=r2=r3=0.14b, and l1=b) is presented below:

EUC=

*3π*9r6_{2}_{1 +}√_{2}_{Gs}_{+}_{13 + 9}√_{2}_{Es}_{+ 2b}2_{r}4_{2}_{5 + 3}√_{2}_{Gs}_{+}_{79 + 53}√_{2}_{Es}

2b2_{9r}4_{26 + 24}√_{2}_{Gs}_{+ 7}_{23 + 16}√_{2}_{Es}_{+ 6b}2_{r}2_{58 + 34}√_{2}_{Gs}_{+}_{407 + 279}√_{2}_{Es}_{+ b}4_{8}_{6 + 5}√_{2}_{Gs}_{+}_{568 + 436}√_{2}_{Es} (14)

*Poisson’s ratio of the unit cell ν*UCcan be found by−q_{q}1_{8}. Hence, by calculating q1and

q8from Equation (10) and substituting them in this relationship, the Poisson’s ratio formula

for the unit cell can be derived. The Poisson’s ratio relationship of the above-mentioned
*specific case (θ*=*ϕ*=0◦, r1=r2=r3=0.14b, and l1=b) can be obtained as follows:

*ϑ*UC=
126 + 5√2b4_{E}
s+ 6b2r2
2Gs+
5 +√2Es
− 9r4_{2G}
s+
5 + 4√2Es
9r4_{26 + 24}√_{2}_{G}_{s}_{+ 7}_{23 + 16}√_{2}_{E}_{s}_{+ 6b}2_{r}2_{58 + 34}√_{2}_{G}_{s}+407 + 279√2Es
+ b4_{8}_{6 + 5}√_{2}_{G}_{s}+568 + 436√2Es
(15)

Evaluating the von Mises stress contours of the FE models with several relative
densities showed that vertices B of struts BD are the most critical points (the points with
the maximum stress) in the structure. The yielding of the unit cell as a whole occurs when
*a point in the unit structure reaches the yield stress of the bulk material σ*ys. Therefore, the

yield stress of the re-entrant unit cell can be obtained by assuming that the structure yielding occurs when the stress at point B of struts BD reaches the yield stress of the bulk material. Because strut BD is influenced by both bending moment and axial force (MDB, FDB), the

*maximum stress (σ*max) in point B of this strut could be calculated as follows:
*σ*max = MDB.r2

I2

+FDB

A2 (16)

where r2, I2, and A2are the maximum distance of the points on the strut cross section from

the neutral axis, area moment of inertia, and cross-sectional area of strut DB, respectively. To obtain the bending moment and axial force in strut DB, all of the lateral deformation and axial elongation of this strut applied by DOFs should be considered. DOFs q5, q6, and

q7apply axial elongation and lateral displacement to ends B and D of this strut. Moreover,

DOF q10applies twist to point D. Eventually, the axial forces at point B of strut BD can be

obtained as follows:

Similarly, the bending moments at point B of strut DB can be obtained as

MDB= (−q5*cos θ*+q7*cos θ*+q6*sin θ*)V2+ (q10)U2 (18)

By substituting FDB and MDBfrom Equations (17) and (18) into Equation (16) and

inserting q5, q6, q7, and q10 from solution of the inverse of Equation (10), the maximum

local yield stress in strut DB can be obtained. For the specific case introduced above
*(θ* = *ϕ* = 0◦, r1 = r2 = r3 = 0.14b, and l1 = b), the relationship can be simplified

as follows:
*σ*max=
F2b3_{r}
2Gs−
1 + 2√2Es
+ 6b2_{r}2
212 + 7√2Gs+ 31
4 + 3√2Es
− 3br3
2Gs+
5 + 4√2Es
+ 18r4
2Gs+
5 + 4√2Es
+ b4
86 + 5√2Gs+
664 + 516√2Es
*36bπr*5_{2}_{1 +}√_{2}_{G}
s+
13 + 9√2Es
+ 8b3* _{πr}*3

_{2}

_{5 + 3}√

_{2}

_{G}s+ 79 + 53√2Es (19)

Because the applied stress equal to the structure yield stress of the re-entrant unit cell
*σ*y,UC*causes the maximum local yield stress σ*max at point B, reaching the bulk material

*yield stress σ*y,s, the normalized yield stress of the unit cell could be obtained by a

*cross-multiply of structure mean stress σ*UC= AFUCUC *and σ*maxon the one hand and the relevant
yield stresses on the other hand, which is

*σ*y,UC
*σ*y,s

= FUC

AUC*.σ*max

= F

4(l1+l3*cos ϕ*−l2*sin θ*)2*.σ*Max

(20) Because the idealized 3D re-entrant structure includes vertical struts (strut AB), the unit cell can be vulnerable to buckling under compressive loading. Strut AB in the unit cell structure can be considered as a column under a pure compressive load, and the critical elastic buckling force of the column can be obtained using the classic Euler’s buckling theory as follows:

Pcritical =
*π*2EsI1

(Kl1)2

(21) By considering strut AB as a clamped column based on the periodic boundary condi-tions, the theoretical K value of the column will be equal to 1 and the critical load of an idealized 3D re-entrant unit cell under compressive load F can be obtained as

Pcritical =
*π*2EsI1

l12

(22)
Because the total load applied to a single unit cell and to strut AB is identical (load F),
by considering the 4(l1+l3*cos ϕ*−l2*sin θ*)2as the cross-sectional area of the unit cell, the

critical buckling stress could be obtained as follows:
*σ*critical =

*π*2EsI1

4(l1+l3*cos ϕ*−l2*sin θ*)2l12

(23) 2.1.5. Effective Lengths

One of the important considerations in deriving the analytical relationships of me-chanical properties of structures is that the struts are connected rigidly to each other at the vertices of structures. Ideally, the struts are connected to each other from their very endpoints (vertices demonstrated in Figure2a), and they do not interact with each other from any other point. However, in practice, when several struts approach a vertex, as the cross-section area of the struts is non-zero, some volumes overlap with each other at the ver-tices, which in turn decreases the effective lengths of struts participating in the deformation of the structure. This phenomenon becomes of much more significance in auxetic lattices because they have very acute angles at the vertices (see, for example, Figures2and8).

**Materials 2021, 14, 993** 16 of 36

* Materials 2021, 14, x FOR PEER REVIEW * 16 of 36

**Figure 8. An additively manufactured specimen with 𝜇 = 0.25 under loading test. **

In this study, the minimum distances between the joints were considered as the ef-fective length of the struts. This definition for efef-fective length was in accordance with what was observed in the stress and strain distribution of the structure obtained from the finite element (FE) results. In the following, the analytical derivation of effective lengths has been presented.

The effective length 𝑙 , can be calculated by subtracting the intersection length be-tween Type-I and Type-II struts from 𝑙 as follows:

𝑙 , = 𝑙 − 𝑟

𝑐𝑜𝑠 𝜃− 𝑟 𝑡𝑎𝑛 𝜃 (24)

The effective length of Type-II strut is calculated by measuring the distance between the intersection of two Type-II struts at point D (struts DB and DE) and the intersection of Type-I and Type-II struts at point B (struts AB and BD), and it can be calculated by sub-tracting the intersecting lengths from 𝑙 as

𝑙 , = 𝑙 − 𝑟

𝑡𝑎𝑛 𝛼 2− 𝑟 𝑡𝑎𝑛 𝜃 − 𝑟

𝑐𝑜𝑠 𝜃 (25)

where 𝛼 is the angle between two Type-II struts.

Similarly, the overlapping of Type-III strut occurs in the intersection of Type-II and Type-III struts at point D (struts DC and DG) and the intersection of two Type-II struts at point C. The effective length can then be calculated by subtracting the intersection lengths from 𝑙 as 𝑙 , = 𝑙 − 𝑟 𝑠𝑖𝑛 𝛼 − 𝑟 𝑡𝑎𝑛 𝛼 − 𝑟 𝑡𝑎𝑛 𝜑 (26)

where 𝛼 is the angle between Type-II and Type-III struts.

By substituting these effective lengths into the stiffness matrix and solving the system of Equation (10), analytical relationships for mechanical properties of the 3D re-entrant unit cell can be obtained.

It is worth noting that the analytical relationships for angles 𝛼 and 𝛼 can be ob-tained as follows:

𝛼 = 𝑎𝑟𝑐𝑐𝑜𝑠 2𝑙 cos 𝜑 + √2𝑙 cos 𝜑 sin 𝜑 + √2𝑙 sin 𝜑 sin 𝜃

2𝑙 (27)

𝛼 = 𝑎𝑟𝑐𝑐𝑜𝑠 𝑙 cos 𝜑 (𝑙 cos 𝜑 + 2𝑙 sin 𝜃)

𝑙 (28)

*2.2. Experimental Tests *

**Figure 8.***An additively manufactured specimen with µ*=0.25 under loading test.

In this study, the minimum distances between the joints were considered as the effective length of the struts. This definition for effective length was in accordance with what was observed in the stress and strain distribution of the structure obtained from the finite element (FE) results. In the following, the analytical derivation of effective lengths has been presented.

The effective length l1,e f f can be calculated by subtracting the intersection length

between Type-I and Type-II struts from l1as follows:

l1,e f f =l1−

r2

*cos θ* −r1*tan θ* (24)

The effective length of Type-II strut is calculated by measuring the distance between the intersection of two Type-II struts at point D (struts DB and DE) and the intersection of Type-I and Type-II struts at point B (struts AB and BD), and it can be calculated by subtracting the intersecting lengths from l2as

l2,e f f =l2− r2

tan*α*2

2

−r2*tan θ*− r1

*cos θ* (25)

*where α*2is the angle between two Type-II struts.

Similarly, the overlapping of Type-III strut occurs in the intersection of Type-II and
Type-III struts at point D (struts DC and DG) and the intersection of two Type-II struts at
point C. The effective length can then be calculated by subtracting the intersection lengths
from l3as
l3,e f f =l3− r2
*sin α*1
− r3
*tan α*1
−r3*tan ϕ* (26)

*where α*1is the angle between Type-II and Type-III struts.

By substituting these effective lengths into the stiffness matrix and solving the system of Equation (10), analytical relationships for mechanical properties of the 3D re-entrant unit cell can be obtained.

*It is worth noting that the analytical relationships for angles α*1*and α*2can be obtained

as follows:
*α*1=arccos 2l3cos
2_{ϕ}_{+}√_{2l}
3*cos ϕ sin ϕ*+
√
2l2*sin ϕ sin θ*
2l2
!
(27)

*α*2=arccos

l3*cos ϕ*(l3*cos ϕ*+2l2*sin θ*)

l22

(28) 2.2. Experimental Tests

A Quantum Generous 3D printer (Persia Company, Iran) with poly-lactic acid (PLA) filaments was used for manufacturing the test specimens. Because the mechanical proper-ties of PLA could be different after the printing process as compared to its properproper-ties in the original filament form, in order to obtain the mechanical properties of the bulk material, three types of cylindrical specimens were manufactured and tested under compressive loading. The cylinders were printed in the horizontal (0◦), vertical (90◦), and inclined (45◦) orientations with respect to the build plate direction. Four specimens were manufactured for each cylinder type (12 specimens in total). All the cylindrical specimens had a nominal length of 20 mm and a diameter of 15 mm.

*Three sets of re-entrant unit cell specimens with five different relative densities µ*=0.1,
0.15, 0.2, 0.25, and 0.3 were manufactured (15 specimens in total), see Figures S4 and S5.
The dimensions of all the re-entrant unit cell specimens were 7.71 × 7.71× 7.71 cm3.
All the specimens (unit cells and cylinders) were manufactured with a layer thickness
of 100 µm and infill density of 100%. Because the forces required for collapsing the
manufactured specimens were in the range of 750 N to 3700 N, to avoid the inaccuracies
caused by the deformation of the test machine itself, all the tests were performed with a
large compression test machine (150 kN) for which the deformation in the machine was
negligible. More information on the effect of deformation of the mechanical test bench can
be found in [59]. The static compression tests were performed using an STM-20 (STANTAM,
Iran) mechanical testing bench with a 20 kN load cell (Figure8). The displacement rate
was set to 0.1 mm/min. The normalized elastic modulus and normalized yield stress of
specimens were obtained from load-displacement graphs, and the Poisson’s ratio of the
unit cells were extracted from the side-view images.

2.3. Numerical Modeling

Two FE models were developed in ANSYS software (Pennsylvania, United States) to calculate the mechanical properties of the re-entrant lattice structures. Because analytical formulas of mechanical properties of unit cells have been derived based on Euler–Bernoulli and Timoshenko beam theories, in the first FE model type, Timoshenko beam elements (3D Quadratic finite strain beam, i.e., beam element Type 189 in ANSYS) were used for discretizing the struts of the unit cell. Timoshenko beam theory takes into account the transverse shear deformation. Each strut was divided into five beam elements. The struts were considered to be rigidly connected to each other at the vertices. The linear elastic material properties of the PLA obtained from the experimental tests were adopted. The elastic modulus, Poisson’s ratio, and yield stress of the beam elements were set to 1.93 GPa, 0.33, and 69 MPa, respectively. Periodic boundary conditions were applied to the FE models. The lowermost nodes of the unit cell at point A2Figure2a) were fully constrained

in all the transitional and rotational directions. The top node of the unit cell at point A1

(Figure2a) was displaced downward, but they were not also allowed to have any horizontal displacement or rotation in any direction (Figure S3).

The second FE model type was developed using volumetric elements. This FE model is expected to better take into account the overlapping effect at the joints on the overall mechanical properties of the structure. Five 3D models of the re-entrant unit cell with geometries almost identical to the geometry of the manufactured specimens (relative densities of 0.1, 0.15, 0.2, 0.25, and 0.3) were constructed. An adaptive fine volumetric mesh was implemented for discretizing the models using tetrahedral 10-node elements (SOLID187 elements in ANSYS) to have a fine mesh at the vertices and efficient larger mesh at the middle of the struts. The finest and most accurate options in ANSYS adaptive meshing, i.e., fine resolution (resolution = 6), slow transition, and fine span angle were chosen. The minimum and maximum element sizes for the lowest-density structure

**Materials 2021, 14, 993** 18 of 36

*(µ*=0.1) were 0.3912 mm and 1.78 mm, respectively. The minimum and maximum element
*sizes for the highest-density structure (µ*=0.3) were 0.5786 mm and 2.45 mm, respectively.
The number of elements in the lowest-density and the highest-density structures was
470,701 and 437,269, respectively. Similar to the beam elements, the elastic modulus and
Poisson’s ratio of 1.93 GPa and 0.33, respectively, were considered for the bulk material
properties. To apply the loading and boundary condition, the lowermost face of the model
(lower cross-sectional face of vertex of the strut in Figure2) was fixed in all the directions
and the top face of the model at the point was displaced downward. The material properties
assigned to the volumetric elements were the same as those used in the first FE model.

In order to calculate the elastic modulus of the FE models, the sum of reaction force(s)
at the lowermost node(s), FUC*, due to the vertical displacement of the top node(s), δ*UC,

was measured and substituted in EUC = FAUCUCL*δ*UCUC, where AUCis the cross-sectional area of
the FE model in the plane normal to the loading direction, and LUCis the length of the FE

structure in the direction parallel to the loading direction.

For obtaining the Poisson’s ratio, the elongation of the structure in the lateral direc-tion (X or Z direcdirec-tion) was divided by the contracdirec-tion of the structure in the Y direcdirec-tion (loading direction).

Eventually, for obtaining the numerical normalized yield stress, the maximum stresses
*(von Mises stress) in strut DB of the unit cell (σ*max) was extracted and inserted into the

equation FUC

AUC*.σ*max.

**3. Results**

In this section, all the obtained analytical, numerical, and experimental results are
presented and compared to each other. To have a better understanding of the main factors
influencing the overall performance of the auxetic lattice structure, the effect of each main
*geometrical parameter of the structure such as relative density, angle θ, and angle ϕ are*
studied individually. Moreover, a lightened unit cell, obtained by eliminating the struts l3

from the general 3D re-entrant unit cell, is introduced and its mechanical properties are presented. More details on the results can be found in Section S.2 of the supplementary materials (Figures S7–S27).

3.1. Effect of Relative Density

According to analytical relationships of mechanical properties of the re-entrant unit
cell obtained in Section2.1, elastic modulus, Poisson’s ratio, and yield stress of the structure
depend on seven geometrical main parameters, namely, r1, r2, r3, l1, l2or l3*, θ, and ϕ. To*

validate the analytical relationships, the mechanical properties of a specific case has been
considered in which all the struts have the same radii (r1 =r2=r3*), angles θ and ϕ are*

considered to be equal to 22.5◦, and l1=b where b is shown in Figure2b. It is worth noting

that all the additively manufactured specimens have also been constructed according to
the above-mentioned geometrical parameters. Effects of variations in the relative density
*of 3D re-entrant unit cell with respect to angles θ and ϕ is shown in Figure S7.*

The analytical (based on Euler–Bernoulli and Timoshenko beam theories), numeri-cal (based on beam and volumetric elements), and experimental results of this case are presented and compared in Figure9. The main take-out of this figure is that both the Euler–Bernoulli and Timoshenko analytical models after consideration of the effective length, the numerical models based on volumetric elements, and the experimental data points have good agreement with respect to each other. On the other hand, the results of both the Euler–Bernoulli and Timoshenko analytical models without consideration of the effective length and the numerical model based on beam elements (rather than volumetric elements) are close to each other but quite far from the experimental data points. As it can be seen in Figure9, the analytical models considering the overlapping effect and the numerical models made from volumetric elements have higher levels of stiffness and yield stress, and lower levels of Poisson’s ratio in comparison with the analytical models without